A One-Piece Lunar Regolith-Bag Garage Prototype Lunar Settlements Symposium Rutgers University June 5, 2007 Gweneth A. Smithers, Mary K. Nehls, Mary A. Hovater, Steven W. EvansNASA/Marshall Space Flight Center, Huntsville, Alabama J. Scott MillerQualis Corporation/Marshall Space Flight Center, Huntsville, Alabama Roy M. Broughton, Jr., David Beale, and Fatma Kilinc-BalciAuburn University, Auburn, Alabama
Why Regolith-Bags? While sandbagging has been a technique on Earth for centuries, more recent years have seen some work on lunar regolith-bag concepts. If NASA is to colonize the Moon and explore the Universe, it will certainly become necessary to use the native materials of planets of residence. Throughout history, communities have always relied on raw materials close at hand. While recent decades (on Earth) have seen a tendency to skirt around this practice with exploitation of “free trade,” transportation realities will force us to revert to historical practice when we colonize other planets. Regolith, properly utilized, can provide thermal insulation and radiation shielding – as well as chemicals necessary for life.
Earthly sandbags have been used For a very long time. There is a village in California with sand-bag “residences.”
Goals • To learn, through materials testing, which materials are suitable for use in construction of a one-piece regolith-bag form to be launched from Earth, landed on the Moon, filled with raw lunar regolith, and used as a functional structure (materials - chosen from a previous literature review - to be tested in conjunction with official lunar regolith simulant). • To successfully design, develop and construct a large one-piece regolith-bag form and fill it with a low-fidelity simulant, producing the Lunar Garage Prototype.
Candidate Fabric Materials • 1. Vectran TM - polyester liquid crystal polymer, (LCP) • 2. Nextel TM - aluminoborosilicate (ceramic) • 3. Gore PTFE TM - expanded polytetrafluoroethylene (PTFE) • 4. Nomex TM - meta-aramid fiber • 5. Twaron TM - para-aramid fiber (used instead of KevlarTM - has similar chemistry); • 6. Zylon TM - a rigid-rod polymer - poly (P-phenylene-2,6-benzobisoxazole), PBO.
Fold Endurance • Folding endurance is unlikely to be a problem for any fabric tested, except Nextel. • Twaron ranked somewhat poorer in fold resistance than the other organic fibers.
Abrasion Testing • The resistance of fabrics was determined on a CSI-Stoll Quartermaster Universal Wear Tester (Custom Scientific Instruments Inc.) by a modification of ASTM D-3885 (flexing and abrasion method). • The resistance to abrasion is affected by many factors: the inherent mechanical properties of the fibers, the dimensions of the fibers, the structure of the yarns, the construction of fabrics and finish type. The resistance of fabrics to abrasion as measured by this method is generally only one of the several factors contributing to durability.
In this test, 3 fabric samples, cut 3 x 8 inches in both warp and filling direction, are subjected to unidirectional reciprocal rubbing over a sandpaper surface, under 5 pounds weight. The sample is placed between the pressure (upper) plate and reciprocating (lower) plate. The lower plate was covered by sand paper (220 Grit). • A 2.5mm thick, soft fabric padding was placed under the sample to provide conformability. The number of cycles is recorded upon failure of the fabric or after 1000 cycles.
Stoll Flex-Abrasion Tester
Abrasion Results • Gore PTFE TM left some little particles on the sand paper surface but the fabric damage was not excessive. • Vectran TM and Twaron TM were in very good condition even after 1000 cycles • Although the failure criteria are somewhat subjective: Nextel TM samples had failed after 350 cycles, and • Nomex TM and Zylon TM fabrics had failed after 500 cycles
JSC Abrasion Test • One bag of each fabric loosely filled bag (of regolith simulant) was placed in the tumbling drum along with regolith simulant on the outside of the bags, • The drum was rotated at 13rpm for 1 hour. • Subsequently, the remaining bags were placed in the drum and were tumbled for 1 hour.
JSC Abrasion Results • Nextel and Gore PTFE showed some damage, but mainly at the seams. • The other fabrics were essentially undamaged.
The Lunar Radiation Environment • Referenced recent natural environment study performed by MSFC EV13 • Lunar surface environment is predominantly • Solar wind (mostly low to mid energy e- and H+) • Cosmic ray environment (Solar Particle Events and Galactic Cosmic Rays) • Impact (although this is not radiation) • Analysis indicates that the dose driver for the bulk material is from solar wind
Radiation Resistance • Vacuum Ultra Violet - VUV • Particle radiation • Gamma radiation • Compare strength before and after radiation.
Three replicate tensile samples Gore PTFE Nextel Vectran Samples were exposed on a 1” (fill) x 4” (warp) area Samples were sent to Auburn post-irradiation for mechanical (tensile) testing One bag specimen constructed of Vectran For impact testing Charged Particle Radiation Exposure
Pre-irradiation Vectran Post-irradiation Vectran Charged Particle Exposures Samples were exposed to a current flux of 1nA/cm² to obtain a total fluence of 3.6E14 e-/cm² at 250 keV e- kinetic energy (30 Mrad dose) Representative samples for total ionizing dose testing Pre-irradiation Vectran bag Post-irradiation Vectran bag
Three replicate tensile samples of Gore PTFE Nextel Vectran Twaron Two replicate tensile samples of Nomex Zylon Each sample was exposed on a 1” (fill) x 2” (warp) area Vacuum Ultraviolet Radiation Exposure
Plate 2 Plate 1 VUV Exposures - Plate distance 39” from deuterium lamp source- Exposures were performed simultaneously with each plate facing 180° apart, directed at a separate lamp- Actual exposure time was 1246 hours- Normally stated acceleration factor is 2.5x (e.g., 3115 solar equivalent hours)
Radiation Exposure Summary • We determined through radiation transport calculations an appropriate Lunar radiation simulation approach for a 10 year total charged particle ionizing dose in three materials • Using the MSFC Combined Environmental Effects Facility we irradiated a total of 10 material samples to an expected 10-year lunar charged particle radiation dose • We irradiated a total of 16 samples with vacuum ultraviolet radiation to at least 3115 equivalent hours of solar VUV exposure
Gamma Radiation ResultsExposure to 10 megarads over one day. Co 60 radiation source
Testing Facility Hypervelocity impact testing was completed on the proposed regolith bag materials at the MSFC EM50 Impact Testing Facility (ITF) using the Micro Light Gas Gun (MLGG). Projectiles used for this testing were 1mm aluminum spheres with average velocities of 7km/s. Each bag was placed in the chamber and aligned with a laser before each test.
Basic bag set up in chamber and laser aligning Each bag is approximately 6”x6”x4” filled in bldg 4493 with Portland cement to represent lunar regolith. Approximate weight of bag is 6.5lbs.
Exposed Vectran (Vectran-R) Penetration dia + damage dia = 4mm
Note: Bag penetration diameters were measured using a hand held scale. No precision measurements were take due to the filled bag shape. Precision measurements could be taken if the bags were emptied carefully as to not disturb the penetration site.
Design Specification The design of this prototype was based on the principles of the classic masonry arch.
Final Design – Construction Template • The fabric consisted of a top Kevlar layer, to which fabric “teeth” were stitched. “Top Connected Bag Configuration” • Construction Template – x-y coordinate of numbered points • Template based on structural analysis techniques for masonry arches (“Funicular Polygon”). • A catenary shape • Pipes attached to frame were used as guides at points 10, 14 and 21.
Concepts That Led to the Design • Vermiculite was chosen to simulate regolith; Its weight on earth/unit volume (density .16-.2 g/cc) is the near that of weight of lunar regolith/unit volume (density .27 g/cc) of any bulk material. • Strength of vermiculite-filled bags depends on vermiculite pressure. At high pressure, the grain interlock, increasing resistance to shearing failure of the vermiculite. Pressure could be generated by • 1) Weight and loads from the structure above. Used for bottom bags. • 2) Packing the bags tightly so they strain the bag, and try to round. Used for top bags. • The “beam” (next slide) demonstrated the advantages of the “top-connected” configuration for erecting of the structure, by being able to support bending loads. • The assumptions used to design a masonry arch were assumed valid for the design the regolith bag arch. These include: 1) No sliding between bags, 2) Only compressive forces are transmitted across brick boundaries (bricks cannot transmit tensile loads), 3) The bricks have infinite compressive strength. • Masonry Arches fail by “hinging”. This was also observed in the regolith bag arch. • The foundation provides the horizontal force at the base. Taller arches are more stable. Build the arch on a frame, then remove the frame.
The Final Garage Structure – A Top-Connected Regolith Bag Arch • Notice top fabric layer and bags (“teeth”). • Fabric made from coated Kevlar • Zippers (other side) for filling • Wooden frame with pipe supports at locations dictated by the construction template • Used 46 of 60 bags
How Bags Were Filled • Series 300 Haupman helical flexible screw conveyor system, with green hopper. • 3” diameter, 12’ helical screw inside pipe had no central shaft, making screw axially flexible, limiting the feed force. This significantly impacted the ability to fill bags with substantial pressure. • The pipe was inserted to the end of the bag and slowly withdrawn as vermicullite filled the bag.
Comments on Final Garage Structure • Notice Pipe no longer supported. • Sagging on right hand side in this view, but still a stable structure. • Sagging here is a result of visible slipping. Bags were just not packed tight enough. Rear View
Conclusions and Recommendations (1)Having completed this initial materials testing program, we recommend that VectranTM (which tested best overall) be carried into the next stage of study. KevlarTM or TwaronTM could also be considered for additional study, but Gore PTFETM , ZylonTM , and NomexTM should be dropped as base material candidates. If Gore PTFETM is considered as an auxiliary material, a higher strength type of Gore PTFETM should be tested. NextelTM should be dropped as a candidate, with the possible exception of its consideration for limited use in any rigid area where it is sandwiched in between other materials (or, if some type of coating could be developed for NextelTM to make it more flex and abrasion resistant and thereby exploit its radiation resistance). (2) The simulated 10-year total ionizing dose we used for radiation exposure worked well, since it showed sensitivity differences in fabric candidates. In future radiation exposure testing, we should test VectranTM at 30-year total ionizing dose, if possible.
Conclusions and Recommendations (3)VectranTM and TwaronTM tested best in the standard abrasion test. These two materials should be tested to failure in the standard abrasion test. They also tested well in the JSC regolith simulant tumble abrasion test, but the duration was not long enough to draw final conclusions, so another tumble test of longer duration is recommended. Also, there is a question about the ability of the simulant (JSC-1) to behave as harshly as the actual material. (4) Although ZylonTM showed superior tensile strength in general, it is not recommended for further consideration due to its inferior abrasion testing performance. (5) VectranTM appears to have high folding endurance; however, a higher number of cycles is recommended for the cryogenic folding test.
Conclusions and Recommendations (6) More extensive hypervelocity impact testing is recommended for VectranTM , the highest overall performer. (7) At this point, we have a "demonstration article," the one-piece lunar regolith-bag garage prototype, standing, on its own, in Building 4493 at MSFC. Work to date indicates that the theory that a regolith-bag arch can behave in much the same manner as the classic masonry arch is valid; however, we have taken only the first step in proving this theory, and other steps are required.
Conclusions and Recommendations (8) Our task team should discuss what a "next phase" would look like, as there are many possible approaches, such as the choice to proceed one small increment at a time, or to look at several "angles" at once. (9) We should consider a study (materials testing program) which looks at using multiple layers of fabric for the regolith-bag pockets. For example, we might look at a two-layered structure, using VectranTM and TwaronTM or KevlarTM . Or, we might look at a three-layered structure, using NextelTM sandwiched in between two layers of VectranTM . (10) We should consider a materials testing program looking at VectranTM as a single layer but with various coatings.
Conclusions and Recommendations (11) We should consider a materials testing program looking at the materials used in the sample prototype section which was produced by Techsphere, Inc. This material was VectranTM on top of which had been laminated a thin layer of aluminum foil. This is the material we wanted to use to make the prototype; however, the cost and the lead time were prohibitive. (12) We should consider what type of customized blended fiber could be used to make a fabric tailored for this application. (13) We should consider the simulated lunar environment to be used for testing materials and structures - ways to improve on procedures used in this work. . We should aim for increasingly higher fidelity lunar environment simulation.